Download presentation

Presentation is loading. Please wait.

Published bySophia Horton Modified over 4 years ago

1
Thomas Chanier ISEN Engineer – PhD student IM2NP, MARSEILLE, France Co-workers : R. Hayn, M. Sargolzaei, I. Opahle, M. Lannoo Thomas Chanier ISEN Engineer – PhD student IM2NP, MARSEILLE, France Co-workers : R. Hayn, M. Sargolzaei, I. Opahle, M. Lannoo PhD defense - 29/08/2008 – Faculté de St-Jérôme, Marseille, France Electronic structure and magnetic properties of II-VI DMS

2
IntroductionIntroduction Failure of Moores law : –The number of transistors / inch² on P chips doubles every two years –Current technology : Based on electron charge Atomic scale : –Quantum nature of the electron –Needed : new science to replace classical micro- electronics Failure of Moores law : –The number of transistors / inch² on P chips doubles every two years –Current technology : Based on electron charge Atomic scale : –Quantum nature of the electron –Needed : new science to replace classical micro- electronics L G <50 nm (~1000 at.) STM image, IBM TEM image http://public.itrs.net/ Fe corral on AuMOS FET d~LG²d~LG²

3
SpintronicsSpintronics SpinFET - Datta and Das, APL 56 665 (1990) –Principals : Rashbas precession –Current challenge : Injection of spin-polarized current in the SC channel –Unsuccessful attempts : S and D in FM metal : weak injection due to conductivity mismatch with SC Schmidt et al., PRB 62 R4790 (2000) Alternative solution for spin injection : DMS : diluted magnetic SC - Classical : SC doped with magnetic ions (TM or rare earth) - New class of DMS ? magnetic intrinsic defects (vacancy, interstitial) Needed : FM at room temperature for spintronic applications SpinFET - Datta and Das, APL 56 665 (1990) –Principals : Rashbas precession –Current challenge : Injection of spin-polarized current in the SC channel –Unsuccessful attempts : S and D in FM metal : weak injection due to conductivity mismatch with SC Schmidt et al., PRB 62 R4790 (2000) Alternative solution for spin injection : DMS : diluted magnetic SC - Classical : SC doped with magnetic ions (TM or rare earth) - New class of DMS ? magnetic intrinsic defects (vacancy, interstitial) Needed : FM at room temperature for spintronic applications Scientific American

4
Basics on II-VI DMS Ref. 1 : Jamieson, J. Phys. Chem. Solids 41 963 Ref. 2 : CRC Handbook of Chemistry and Physics Ref. 3 : Sabine, Acta Cryst. B 25 2254 Ref. 4 : Reeber, JAP 38 1531 Ref. 5 : Yim, J. Electr Soc Sol-St.Sci. Tech 119 381 Host SC : covalent bonds Zn 2+ A 2- Substitutional impurity : TM 2+ config. : [Ar] 3d n 4s 0 : - for Co, n=7 S = 3/2 - for Mn, n=5 S = 5/2 ZB : only 1 NN exchange integral J NN W : 2 NN exch. Int. : in-plane J in & out-of-plane J out ZB W

5
State of the art l l FM prediction for ZnTMO : - Sato et al., Physica E 10 251 (2001) LSDA : FM J NN in ZnCoO - Dietl et al., PRB 63 195205 (2001) Zener model, p-type ZnMnO AFM & FM competition for ZnCoO & AFM for ZnMnO : - Lee et al., PRB 69 085205 (2004) - Sluiter et al., PRL 94 187204 (2005) LSDA + pseudopotential BUT : in contrast to experiments Our study : AFM NN exchange constants - LSDA+U : Hubbard-type correction to LSDA AFM J NN T. Chanier et al., PRB 73 134418 (2006) - Predictions confirmed: AFM interactions in ZnCoO, P. Sati et al., PRL 98 137204 (2007) Dietl (2001) Sati (2007) LSDA+U

6
d-d exchange Hamiltonian Heisenberg Hamiltonian : J > 0 FM J < 0 AFM Comparison of E in the Heisenberg model with E Total obtained from FM and AFM First-principle calculations : chain : pair : Where S T = 2S the total spin for two magnetic impurities of spin S First-principle calculations : FPLO : full potential local orbital approximation (Koepernic et al., PRB 59 1743) LSDA : Perdew-Wang 92 Vxc functional (Perdew and Wang, PRB 45 13244) LSDA+U : atomic limit scheme (Anisimov et al., PRB 44 943) No additional carrier codoping Heisenberg Hamiltonian : J > 0 FM J < 0 AFM Comparison of E in the Heisenberg model with E Total obtained from FM and AFM First-principle calculations : chain : pair : Where S T = 2S the total spin for two magnetic impurities of spin S First-principle calculations : FPLO : full potential local orbital approximation (Koepernic et al., PRB 59 1743) LSDA : Perdew-Wang 92 Vxc functional (Perdew and Wang, PRB 45 13244) LSDA+U : atomic limit scheme (Anisimov et al., PRB 44 943) No additional carrier codoping

7
Supercell approach

8
Exchange constants for ZnO:Co LSDA : competition between AFM and FM interactions for the two type of NN in constrast to exp. Necessity of better taking into account the strong electron correlation in the TM 3d-shell LSDA+U : AFM exchange constants for the two type of NN in quantitative agreement with exp. We use the same Slater parameters as those of CoO Two realistic values for U = 6 and 8 eV Ref. : Anisimov et al., PRB 44 943 (1991) Our values : J in = -1.7 ± 0.3 meV, J out = -0.8 ± 0.3 meV Experiments : –Tcw of magnetic susceptibility : J ave = -33 K = -2.8 meV –INS : J in = -2.0 meV, J out = - 0.7 meV Ref. : Yoon et al., JAP 93 7879 (2003), Stepanov, private comm. (2008) LSDA : competition between AFM and FM interactions for the two type of NN in constrast to exp. Necessity of better taking into account the strong electron correlation in the TM 3d-shell LSDA+U : AFM exchange constants for the two type of NN in quantitative agreement with exp. We use the same Slater parameters as those of CoO Two realistic values for U = 6 and 8 eV Ref. : Anisimov et al., PRB 44 943 (1991) Our values : J in = -1.7 ± 0.3 meV, J out = -0.8 ± 0.3 meV Experiments : –Tcw of magnetic susceptibility : J ave = -33 K = -2.8 meV –INS : J in = -2.0 meV, J out = - 0.7 meV Ref. : Yoon et al., JAP 93 7879 (2003), Stepanov, private comm. (2008) Ref. 1 : Lee and Chang, PRB 69 085205 (2004) (LSDA, pseudopotential) Ref. 2 : Sluiter et al., PRL 94 187204 (2005) (LSDA, pseudopotential)

9
Exchange constants for ZnO:Mn LSDA : underestimation of AFM exchange constants in either type of NN LSDA+U : AFM exchange constants in quantitative agreement with experiments (SP of MnO, U = 6 & 8 eV) Our values : J in = -1.8 ± 0.2 meV, J out = -1.1 ± 0.2 meV Experimental values : two values of J (MST) J 1 = -2.08 meV, J 2 = -1.56 meV Ref. : Gratens et al., PRB 69 125209 (2004) Ref. 2 : Sluiter et al., PRL 94 187204 (2005) LSDA : underestimation of AFM exchange constants in either type of NN LSDA+U : AFM exchange constants in quantitative agreement with experiments (SP of MnO, U = 6 & 8 eV) Our values : J in = -1.8 ± 0.2 meV, J out = -1.1 ± 0.2 meV Experimental values : two values of J (MST) J 1 = -2.08 meV, J 2 = -1.56 meV Ref. : Gratens et al., PRB 69 125209 (2004) Ref. 2 : Sluiter et al., PRL 94 187204 (2005)

10
Spin density Co-O-Co plane, in-plane NN Co-O-Co plane, out-of-plane NN

11
J NN for ZB II-VI DMS Chemical trends of J NN : Supercells TM 2 Zn 6 A 8 (ZB) A II B VI :Mn - U from Ref. : Gunnarson et al., PRB 40 10407 (1989) - Charge transfer from FPLO : A II B VI :Mn

12
sp-d exchange constants Chemical trends of N and N : Supercells TMZn 3 A 4 (ZB) –Mean Field Approx. : With N the cation concentration sp-d exch cst for CBE and VBH at Chemical trends of N and N : Supercells TMZn 3 A 4 (ZB) –Mean Field Approx. : With N the cation concentration sp-d exch cst for CBE and VBH at

13
LSDA+U DOS

16
LSDA DOS

17
Main features of DOS The upper VB is formed by a semi-circle of width W LSDA : BS & inverted FM VB spin splitting E v = E v - E v > 0 –too high position of TM 3d level, always a bound state LSDA+U : formation of a BS & FM E v if V pd > V pd –If U, the occupied 3d levels are shifted by ~ -U 2 from VBM, 0 = E BS -E v –Hyp. : V pd f(U) –mm The upper VB is formed by a semi-circle of width W LSDA : BS & inverted FM VB spin splitting E v = E v - E v > 0 –too high position of TM 3d level, always a bound state LSDA+U : formation of a BS & FM E v if V pd > V pd –If U, the occupied 3d levels are shifted by ~ -U 2 from VBM, 0 = E BS -E v –Hyp. : V pd f(U) –mm c l

18
Analytical model Bethe Lattice Model : - TB Hamiltonian : - Basis set : - Hamiltonian matrix : - Local Creen Funct. : Bethe Lattice Model : - TB Hamiltonian : - Basis set : - Hamiltonian matrix : - Local Creen Funct. : (t 2g 3d orb. for TM 2+ ) (t 2 p orb. for A 2- )

19
ResolutionResolution Host Green function Local Green function (i)No bound state : f 0 < a & | 0 | < |a-f 0 | (ii)A bound state out of continuum : f 0 > a & | 0 | > |a-f 0 | (iii)2 bound states on both side of the continuum : f 0 > a & | 0 | < |a-f 0 | Host Green function Local Green function (i)No bound state : f 0 < a & | 0 | < |a-f 0 | (ii)A bound state out of continuum : f 0 > a & | 0 | > |a-f 0 | (iii)2 bound states on both side of the continuum : f 0 > a & | 0 | < |a-f 0 | Vpd = 0.90 eV a = 2 eV, 0 = 1 eV Vpd = 0.90 eV

20
ResolutionResolution Host Green function Local Green function (i)No bound state : f 0 < a & | 0 | < |a-f 0 | (ii)A bound state out of continuum : f 0 > a & | 0 | > |a-f 0 | (iii)2 bound states on both side of the continuum : f 0 > a & | 0 | < |a-f 0 | Host Green function Local Green function (i)No bound state : f 0 < a & | 0 | < |a-f 0 | (ii)A bound state out of continuum : f 0 > a & | 0 | > |a-f 0 | (iii)2 bound states on both side of the continuum : f 0 > a & | 0 | < |a-f 0 | Vpd = 0.90 eV a = 2 eV, 0 = 1 eV Vpd = 0.90 eV

21
ResolutionResolution Host Green function Local Green function (i)No bound state : f 0 < a & | 0 | < |a-f 0 | (ii)A bound state out of continuum : f 0 > a & | 0 | > |a-f 0 | (iii)2 bound states on both side of the continuum : f 0 > a & | 0 | < |a-f 0 | Host Green function Local Green function (i)No bound state : f 0 < a & | 0 | < |a-f 0 | (ii)A bound state out of continuum : f 0 > a & | 0 | > |a-f 0 | (iii)2 bound states on both side of the continuum : f 0 > a & | 0 | < |a-f 0 | a = 2 eV, 0 = 1 eV Vpd = 0.90 eV

22
Formation of a Zhang-Rice Singlet Condition of formation of a bound state : - Necessary condition for a BS : f 0 > a=W/2 & 0 not too deep - for ZnO:TM : Two bound states : Condition of formation of a bound state : - Necessary condition for a BS : f 0 > a=W/2 & 0 not too deep - for ZnO:TM : Two bound states :

23
ResultsResults Curve fitting - Results : - Supercell MnZn 31 O 32 : - Harrisons parametrization : Curve fitting - Results : - Supercell MnZn 31 O 32 : - Harrisons parametrization :

24
V pd for Host II-VI SC - Host SC DOS- Critical hybridization param. : - Harrisons parametrization : - Host SC DOS- Critical hybridization param. : - Harrisons parametrization : c

25
Vacancy in II-VI SC : ab initio study - Basis set :- NN relaxation : - Electronic structure : - LSDA results : E = E LDA -E LSDA Zn 4 A 3 calc. : Neutral anion vacancy is non-magnetic - Basis set :- NN relaxation : - Electronic structure : - LSDA results : E = E LDA -E LSDA Zn 4 A 3 calc. : Neutral anion vacancy is non-magnetic

26
Analytical model Molecular cluster model : - sp 3 molecular orbitals : i (i=1..4) - Hamiltonian : Group Theory : SALC of i - monoelectronic states : A 1 and T 2 representations - polyelectronic states : direct product group Molecular cluster model : - sp 3 molecular orbitals : i (i=1..4) - Hamiltonian : Group Theory : SALC of i - monoelectronic states : A 1 and T 2 representations - polyelectronic states : direct product group

27
ResultsResults Monoparticule eigenenergies : Biparticle eigenenergies : = -4 & 4 eV, U = 4 eV, V = 1 eV V Zn 0 in ZnO : S = 1 state characterized by EPR Ref. : D. Galland et al., Phys. Lett. 33A, 1 (1970) Monoparticule eigenenergies : Biparticle eigenenergies : = -4 & 4 eV, U = 4 eV, V = 1 eV V Zn 0 in ZnO : S = 1 state characterized by EPR Ref. : D. Galland et al., Phys. Lett. 33A, 1 (1970) V A 0 in ZnO, S = 0 V Zn 0 in ZnO, S = 1

28
ConclusionConclusion Mn- and Co-doped DMS –Necessity of taking into account the strong electron correlation on the TM 3d shell. –The LSDA+U exchange constants are in quantitative agreement with experiments. –Importance of the hybridation parameter V pd to describe correctly the DOS of DMS. Single vacancy in II-VI SC –Neutral cation vacancy in more ionic ZnO carries a spin S = 1 in agreement with experiments. –This state is quasi-degenerate with a S = 0 state in other less ionic II-VI SC. –Neutral anion vacancy is non-magnetic. Publications : T. Chanier et al., PRB 73 134418 (2006) ; T. Chanier et al., PRL 100 026405 (2008) Mn- and Co-doped DMS –Necessity of taking into account the strong electron correlation on the TM 3d shell. –The LSDA+U exchange constants are in quantitative agreement with experiments. –Importance of the hybridation parameter V pd to describe correctly the DOS of DMS. Single vacancy in II-VI SC –Neutral cation vacancy in more ionic ZnO carries a spin S = 1 in agreement with experiments. –This state is quasi-degenerate with a S = 0 state in other less ionic II-VI SC. –Neutral anion vacancy is non-magnetic. Publications : T. Chanier et al., PRB 73 134418 (2006) ; T. Chanier et al., PRL 100 026405 (2008)

Similar presentations

OK

FZU 30.5.061 Comparison of Mn doped GaAs, ZnSe, and LiZnAs dilute magnetic semiconductors J.Mašek, J. Kudrnovský, F. Máca, and T. Jungwirth.

FZU 30.5.061 Comparison of Mn doped GaAs, ZnSe, and LiZnAs dilute magnetic semiconductors J.Mašek, J. Kudrnovský, F. Máca, and T. Jungwirth.

© 2018 SlidePlayer.com Inc.

All rights reserved.

To make this website work, we log user data and share it with processors. To use this website, you must agree to our Privacy Policy, including cookie policy.

Ads by Google